 
data_RWJTI
 
_audit_creation_method            SHELXL-2013
_chemical_name_systematic
;
 ?
;
#===============================================================================
# 1. SUBMISSION DETAILS
_publ_contact_author_name      'Prof. Dr. Jin-Xiao Mi'
_publ_contact_author_address
;
Department of Materials Science and Engineering
College of Materials,
Xiamen University,
Xiamen 361005, Fujian Province
People's Republic of China
;
_publ_contact_author_phone     '0086-13696905136'
_publ_contact_author_fax       '0086-592-2183937'
_publ_contact_author_email     'jxmi@xmu.edu.cn'
_publ_requested_journal         ?
_publ_requested_category        ?
_publ_requested_coeditor_name   ?
_publ_contact_letter
;
Jan 10, 2015

Please consider this CIF submission for deposit ICSD. 
All authors have seen and approved this submission. 
The authors acknowledge the conditions of publication.

The CIF has passed the enCIFer(V1.1) checking.

Jin-Xiao Mi
;
#===============================================================================


_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'F12 H21.10 K2.97 Mn6 Na8 O41.03 P8 Ti' 
_chemical_formula_weight          1831.03

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0362   0.0249
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'K'  'K'   0.2009   0.2494
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mn'  'Mn'   0.3368   0.7283
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ti'  'Ti'   0.2776   0.4457
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P'  'P'   0.1023   0.0942
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'F'  'F'   0.0171   0.0103
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       cubic
_space_group_IT_number            202
_space_group_name_H-M_alt         'F m -3'
_space_group_name_Hall            '-F 2 2 3'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-x, -y, z'
 '-x, y, -z'
 'x, -y, -z'
 'z, x, y'
 'z, -x, -y'
 '-z, -x, y'
 '-z, x, -y'
 'y, z, x'
 '-y, z, -x'
 'y, -z, -x'
 '-y, -z, x'
 'x, y+1/2, z+1/2'
 '-x, -y+1/2, z+1/2'
 '-x, y+1/2, -z+1/2'
 'x, -y+1/2, -z+1/2'
 'z, x+1/2, y+1/2'
 'z, -x+1/2, -y+1/2'
 '-z, -x+1/2, y+1/2'
 '-z, x+1/2, -y+1/2'
 'y, z+1/2, x+1/2'
 '-y, z+1/2, -x+1/2'
 'y, -z+1/2, -x+1/2'
 '-y, -z+1/2, x+1/2'
 'x+1/2, y, z+1/2'
 '-x+1/2, -y, z+1/2'
 '-x+1/2, y, -z+1/2'
 'x+1/2, -y, -z+1/2'
 'z+1/2, x, y+1/2'
 'z+1/2, -x, -y+1/2'
 '-z+1/2, -x, y+1/2'
 '-z+1/2, x, -y+1/2'
 'y+1/2, z, x+1/2'
 '-y+1/2, z, -x+1/2'
 'y+1/2, -z, -x+1/2'
 '-y+1/2, -z, x+1/2'
 'x+1/2, y+1/2, z'
 '-x+1/2, -y+1/2, z'
 '-x+1/2, y+1/2, -z'
 'x+1/2, -y+1/2, -z'
 'z+1/2, x+1/2, y'
 'z+1/2, -x+1/2, -y'
 '-z+1/2, -x+1/2, y'
 '-z+1/2, x+1/2, -y'
 'y+1/2, z+1/2, x'
 '-y+1/2, z+1/2, -x'
 'y+1/2, -z+1/2, -x'
 '-y+1/2, -z+1/2, x'
 '-x, -y, -z'
 'x, y, -z'
 'x, -y, z'
 '-x, y, z'
 '-z, -x, -y'
 '-z, x, y'
 'z, x, -y'
 'z, -x, y'
 '-y, -z, -x'
 'y, -z, x'
 '-y, z, x'
 'y, z, -x'
 '-x, -y+1/2, -z+1/2'
 'x, y+1/2, -z+1/2'
 'x, -y+1/2, z+1/2'
 '-x, y+1/2, z+1/2'
 '-z, -x+1/2, -y+1/2'
 '-z, x+1/2, y+1/2'
 'z, x+1/2, -y+1/2'
 'z, -x+1/2, y+1/2'
 '-y, -z+1/2, -x+1/2'
 'y, -z+1/2, x+1/2'
 '-y, z+1/2, x+1/2'
 'y, z+1/2, -x+1/2'
 '-x+1/2, -y, -z+1/2'
 'x+1/2, y, -z+1/2'
 'x+1/2, -y, z+1/2'
 '-x+1/2, y, z+1/2'
 '-z+1/2, -x, -y+1/2'
 '-z+1/2, x, y+1/2'
 'z+1/2, x, -y+1/2'
 'z+1/2, -x, y+1/2'
 '-y+1/2, -z, -x+1/2'
 'y+1/2, -z, x+1/2'
 '-y+1/2, z, x+1/2'
 'y+1/2, z, -x+1/2'
 '-x+1/2, -y+1/2, -z'
 'x+1/2, y+1/2, -z'
 'x+1/2, -y+1/2, z'
 '-x+1/2, y+1/2, z'
 '-z+1/2, -x+1/2, -y'
 '-z+1/2, x+1/2, y'
 'z+1/2, x+1/2, -y'
 'z+1/2, -x+1/2, y'
 '-y+1/2, -z+1/2, -x'
 'y+1/2, -z+1/2, x'
 '-y+1/2, z+1/2, x'
 'y+1/2, z+1/2, -x'
 
_cell_length_a                    16.0001(2)
_cell_length_b                    16.0001(2)
_cell_length_c                    16.0001(2)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 90
_cell_volume                      4096.05
_cell_formula_units_Z             4
_cell_measurement_temperature     173(2)
_cell_measurement_reflns_used     1180 
_cell_measurement_theta_min       3.59 
_cell_measurement_theta_max       29.073 
 
_exptl_crystal_description        'Octahedra' 
_exptl_crystal_colour             'rosy-red' 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_method     ?              
_exptl_crystal_density_diffrn     2.969          
_exptl_crystal_F_000              3575
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.320
_exptl_crystal_size_mid           0.320
_exptl_crystal_size_min           0.320
_exptl_absorpt_coefficient_mu     2.858
_shelx_estimated_absorpt_T_min    0.462
_shelx_estimated_absorpt_T_max    0.462
_exptl_absorpt_correction_type    'multi-scan'  
_exptl_absorpt_correction_T_min   0.59606 
_exptl_absorpt_correction_T_max   1.00000 
_exptl_absorpt_process_details    ? 
 
_exptl_special_details
;
 CrysAlisPro, Agilent Technologies,
Version 1.171.36.24 (release 03-12-2012 CrysAlis171 .NET)
(compiled Dec  3 2012,18:21:49)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
 
_diffrn_ambient_temperature       173(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_radiation_source 'Enhance (Mo) X-ray Source'
_diffrn_radiation_monochromator 'graphite'
_diffrn_measurement_device_type 'Xcalibur, Sapphire3, Gemini ultra'
_diffrn_measurement_method        
;
86 images, omega -49.00 - 37.00, Δω=1.0°, theta -22.8497, 
                                      kappa 38.00, Phi -90.0
 32 images, omega -10.00 - 22.00, Δω=1.0°, theta -22.8497, 
                                      kappa 19.00, Phi 150.0
;
_diffrn_detector_area_resol_mean 16.1903
_diffrn_reflns_number             2364
_diffrn_reflns_av_unetI/netI      0.0397
_diffrn_reflns_av_R_equivalents   0.0416
_diffrn_reflns_limit_h_min        -21
_diffrn_reflns_limit_h_max        22
_diffrn_reflns_limit_k_min        -20
_diffrn_reflns_limit_k_max        15
_diffrn_reflns_limit_l_min        -21
_diffrn_reflns_limit_l_max        8
_diffrn_reflns_theta_min          3.602
_diffrn_reflns_theta_max          29.745
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.915
_diffrn_measured_fraction_theta_full  0.992
_diffrn_reflns_Laue_measured_fraction_max    0.915
_diffrn_reflns_Laue_measured_fraction_full   0.992
_diffrn_reflns_point_group_measured_fraction_max   0.915
_diffrn_reflns_point_group_measured_fraction_full  0.992
_reflns_number_total              495
_reflns_number_gt                 409
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection        'CrysAlisPro, Agilent Technologies, 2012)'
_computing_cell_refinement        'CrysAlisPro, Agilent Technologies, 2012)'
_computing_data_reduction         'CrysAlisPro, Agilent Technologies, 2012)'
_computing_structure_solution     'SHELXL-2013 (Sheldrick, 2013)' 
_computing_structure_refinement   'SHELXL-2013 (Sheldrick, 2013)'
_computing_molecular_graphics     
'DIAMOND (Brandenburg, 2011) & ATOMS (Dowty, 2004)'   
_computing_publication_material   'SHELXL-2013 (Sheldrick, 2013)'
 
_refine_special_details
;
 ?
;
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
;
 w=1/[σ²(Fo²)+(0.0535P)²+8.1128P]
 where P=(Fo²+2Fc²)/3
;
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      SHELXL
_refine_ls_extinction_coef        0.00051(10)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
_refine_ls_number_reflns          495
_refine_ls_number_parameters      55
_refine_ls_number_restraints      19
_refine_ls_R_factor_all           0.0426
_refine_ls_R_factor_gt            0.0365
_refine_ls_wR_factor_ref          0.1118
_refine_ls_wR_factor_gt           0.1071
_refine_ls_goodness_of_fit_ref    1.144
_refine_ls_restrained_S_all       1.134
_refine_ls_shift/su_max           0.002
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Mn1 Mn 0.5000 0.7500 0.7500 0.0155(4) Uani 1 4 d S T P . .
Ti1 Ti 0.5000 0.5000 0.5000 0.0158(6) Uani 1 24 d S T P . .
P1 P 0.35264(6) 0.64736(6) 0.85264(6) 0.0218(5) Uani 1 3 d S T P . .
Na1 Na 0.37162(10) 0.62838(10) 0.62838(10) 0.0284(7) Uani 1 3 d S T P . .
K1 K 0.5000 0.5000 0.77971(15) 0.0187(8) Uani 0.494(13) 4 d S T P . .
OW1 O 0.5000 0.5000 0.77971(15) 0.0187(8) Uani 0.506(13) 4 d S T P . .
F1 F 0.5000 0.64556(16) 0.70568(18) 0.0233(7) Uani 1 2 d S T P . .
O1 O 0.33511(14) 0.59339(16) 0.77803(15) 0.0252(6) Uani 1 1 d . . . . .
O2 O 0.40967(14) 0.59033(14) 0.90967(14) 0.0248(9) Uani 1 3 d S T P . .
O31 O 0.5000 0.5000 0.614(3) 0.015(7) Uani 0.201(3) 4 d S TU P . .
O32 O 0.5333(13) 0.5000 0.6113(13) 0.036(4) Uani 0.2633(16) 2 d S TU P . .
O33 O 0.5000 0.462(2) 0.6060(18) 0.027(7) Uani 0.1364(16) 2 d S TU P . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Mn1 F1 1.815(3) 61_666 ?
Mn1 F1 1.815(3) . ?
Mn1 O1 2.071(2) 70_565 ?
Mn1 O1 2.071(2) 10_656 ?
Mn1 O1 2.071(2) 60_556 ?
Mn1 O1 2.071(2) 24_665 ?
Mn1 Na1 3.4340(8) 61_666 ?
Mn1 Na1 3.4340(8) 16_566 ?
Mn1 Na1 3.4340(8) 52_655 ?
Mn1 Na1 3.4340(8) . ?
Mn1 K1 4.0282(3) 9 ?
Mn1 K1 4.0282(3) 69_666 ?
Ti1 O33 1.80(3) 50_556 ?
Ti1 O33 1.80(3) 2_665 ?
Ti1 O33 1.80(3) 58_565 ?
Ti1 O33 1.80(3) 10_656 ?
Ti1 O33 1.80(3) 54_655 ?
Ti1 O33 1.80(3) 6_566 ?
Ti1 O33 1.80(3) 57_666 ?
Ti1 O33 1.80(3) 9 ?
Ti1 O33 1.80(3) 53_666 ?
Ti1 O33 1.80(3) 5 ?
Ti1 O33 1.80(3) 49_666 ?
Ti1 O33 1.80(3) . ?
P1 O1 1.500(2) 24_665 ?
P1 O1 1.500(2) 30_466 ?
P1 O1 1.500(2) . ?
P1 O2 1.581(4) . ?
P1 K1 3.5327(12) . ?
P1 K1 3.5327(12) 69_666 ?
P1 K1 3.5327(12) 29_455 ?
Na1 F1 2.4135(15) 54_655 ?
Na1 F1 2.4135(15) 10_656 ?
Na1 F1 2.4135(15) . ?
Na1 O1 2.527(3) . ?
Na1 O1 2.527(3) 10_656 ?
Na1 O1 2.527(3) 7_665 ?
Na1 O33 2.536(17) 53_666 ?
Na1 O33 2.536(17) 9 ?
Na1 O33 2.536(17) 2_665 ?
Na1 O32 2.571(12) 54_655 ?
Na1 O32 2.571(12) 2_665 ?
Na1 O32 2.571(12) 9 ?
K1 F1 2.613(3) . ?
K1 F1 2.613(3) 2_665 ?
K1 O31 2.65(4) . ?
K1 O32 2.75(2) . ?
K1 O32 2.75(2) 2_665 ?
K1 O33 2.85(3) . ?
K1 O33 2.85(3) 2_665 ?
K1 O2 2.9157(18) . ?
K1 O2 2.9157(18) 52_655 ?
K1 O2 2.9157(18) 2_665 ?
K1 O2 2.9157(18) 51_565 ?
K1 O1 3.032(2) . ?
F1 Na1 2.4135(15) 52_655 ?
O1 Mn1 2.071(2) 30_466 ?
O2 K1 2.9157(18) 69_666 ?
O2 K1 2.9157(18) 29_455 ?
O31 O32 0.53(2) 2_665 ?
O31 O32 0.53(2) . ?
O31 O33 0.62(3) . ?
O31 O33 0.62(3) 2_665 ?
O31 Na1 2.914(4) 52_655 ?
O31 Na1 2.914(4) 51_565 ?
O31 Na1 2.914(4) 2_665 ?
O32 O33 0.81(2) . ?
O32 O33 0.81(2) 2_665 ?
O32 O32 1.06(4) 2_665 ?
O32 O33 1.65(3) 6_566 ?
O32 Na1 2.571(12) 52_655 ?
O32 Na1 2.571(12) 2_665 ?
O33 O32 0.81(2) 2_665 ?
O33 O33 1.22(6) 2_665 ?
O33 O32 1.65(3) 58_565 ?
O33 Na1 2.537(17) 51_565 ?
O33 Na1 2.537(17) 2_665 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
F1 Mn1 F1 180.0 61_666 . ?
F1 Mn1 O1 86.70(9) 61_666 70_565 ?
F1 Mn1 O1 93.30(9) . 70_565 ?
F1 Mn1 O1 93.30(9) 61_666 10_656 ?
F1 Mn1 O1 86.70(9) . 10_656 ?
O1 Mn1 O1 180.0 70_565 10_656 ?
F1 Mn1 O1 93.30(9) 61_666 60_556 ?
F1 Mn1 O1 86.70(9) . 60_556 ?
O1 Mn1 O1 87.63(14) 70_565 60_556 ?
O1 Mn1 O1 92.37(14) 10_656 60_556 ?
F1 Mn1 O1 86.70(9) 61_666 24_665 ?
F1 Mn1 O1 93.30(9) . 24_665 ?
O1 Mn1 O1 92.37(14) 70_565 24_665 ?
O1 Mn1 O1 87.63(14) 10_656 24_665 ?
O1 Mn1 O1 180.0 60_556 24_665 ?
F1 Mn1 Na1 42.01(5) 61_666 61_666 ?
F1 Mn1 Na1 137.98(5) . 61_666 ?
O1 Mn1 Na1 47.04(7) 70_565 61_666 ?
O1 Mn1 Na1 132.96(7) 10_656 61_666 ?
O1 Mn1 Na1 79.53(7) 60_556 61_666 ?
O1 Mn1 Na1 100.47(7) 24_665 61_666 ?
F1 Mn1 Na1 42.01(5) 61_666 16_566 ?
F1 Mn1 Na1 137.98(5) . 16_566 ?
O1 Mn1 Na1 100.47(7) 70_565 16_566 ?
O1 Mn1 Na1 79.53(7) 10_656 16_566 ?
O1 Mn1 Na1 132.96(7) 60_556 16_566 ?
O1 Mn1 Na1 47.04(7) 24_665 16_566 ?
Na1 Mn1 Na1 73.48(8) 61_666 16_566 ?
F1 Mn1 Na1 137.99(5) 61_666 52_655 ?
F1 Mn1 Na1 42.02(5) . 52_655 ?
O1 Mn1 Na1 79.53(7) 70_565 52_655 ?
O1 Mn1 Na1 100.47(7) 10_656 52_655 ?
O1 Mn1 Na1 47.04(7) 60_556 52_655 ?
O1 Mn1 Na1 132.96(7) 24_665 52_655 ?
Na1 Mn1 Na1 106.52(8) 61_666 52_655 ?
Na1 Mn1 Na1 180.0 16_566 52_655 ?
F1 Mn1 Na1 137.99(5) 61_666 . ?
F1 Mn1 Na1 42.01(5) . . ?
O1 Mn1 Na1 132.96(7) 70_565 . ?
O1 Mn1 Na1 47.04(7) 10_656 . ?
O1 Mn1 Na1 100.47(7) 60_556 . ?
O1 Mn1 Na1 79.53(7) 24_665 . ?
Na1 Mn1 Na1 180.0 61_666 . ?
Na1 Mn1 Na1 106.52(8) 16_566 . ?
Na1 Mn1 Na1 73.48(8) 52_655 . ?
F1 Mn1 K1 106.22(9) 61_666 9 ?
F1 Mn1 K1 73.78(9) . 9 ?
O1 Mn1 K1 132.73(7) 70_565 9 ?
O1 Mn1 K1 47.27(7) 10_656 9 ?
O1 Mn1 K1 47.27(7) 60_556 9 ?
O1 Mn1 K1 132.73(7) 24_665 9 ?
Na1 Mn1 K1 119.72(3) 61_666 9 ?
Na1 Mn1 K1 119.72(3) 16_566 9 ?
Na1 Mn1 K1 60.28(3) 52_655 9 ?
Na1 Mn1 K1 60.28(3) . 9 ?
F1 Mn1 K1 73.78(9) 61_666 69_666 ?
F1 Mn1 K1 106.22(9) . 69_666 ?
O1 Mn1 K1 47.27(7) 70_565 69_666 ?
O1 Mn1 K1 132.73(7) 10_656 69_666 ?
O1 Mn1 K1 132.73(7) 60_556 69_666 ?
O1 Mn1 K1 47.27(7) 24_665 69_666 ?
Na1 Mn1 K1 60.28(3) 61_666 69_666 ?
Na1 Mn1 K1 60.28(3) 16_566 69_666 ?
Na1 Mn1 K1 119.72(3) 52_655 69_666 ?
Na1 Mn1 K1 119.72(3) . 69_666 ?
K1 Mn1 K1 180.0 9 69_666 ?
O33 Ti1 O33 180.0 50_556 2_665 ?
O33 Ti1 O33 71.4(9) 50_556 58_565 ?
O33 Ti1 O33 108.6(9) 2_665 58_565 ?
O33 Ti1 O33 108.6(9) 50_556 10_656 ?
O33 Ti1 O33 71.4(9) 2_665 10_656 ?
O33 Ti1 O33 180.0 58_565 10_656 ?
O33 Ti1 O33 71.4(9) 50_556 54_655 ?
O33 Ti1 O33 108.6(9) 2_665 54_655 ?
O33 Ti1 O33 71.4(9) 58_565 54_655 ?
O33 Ti1 O33 108.6(9) 10_656 54_655 ?
O33 Ti1 O33 108.6(9) 50_556 6_566 ?
O33 Ti1 O33 71.4(9) 2_665 6_566 ?
O33 Ti1 O33 108.6(9) 58_565 6_566 ?
O33 Ti1 O33 71.4(9) 10_656 6_566 ?
O33 Ti1 O33 180.0 54_655 6_566 ?
O33 Ti1 O33 71.4(9) 50_556 57_666 ?
O33 Ti1 O33 108.6(9) 2_665 57_666 ?
O33 Ti1 O33 40(2) 58_565 57_666 ?
O33 Ti1 O33 140(2) 10_656 57_666 ?
O33 Ti1 O33 108.6(9) 54_655 57_666 ?
O33 Ti1 O33 71.4(9) 6_566 57_666 ?
O33 Ti1 O33 108.6(9) 50_556 9 ?
O33 Ti1 O33 71.4(9) 2_665 9 ?
O33 Ti1 O33 140(2) 58_565 9 ?
O33 Ti1 O33 40(2) 10_656 9 ?
O33 Ti1 O33 71.4(9) 54_655 9 ?
O33 Ti1 O33 108.6(9) 6_566 9 ?
O33 Ti1 O33 180.0 57_666 9 ?
O33 Ti1 O33 108.6(9) 50_556 53_666 ?
O33 Ti1 O33 71.4(9) 2_665 53_666 ?
O33 Ti1 O33 71.4(9) 58_565 53_666 ?
O33 Ti1 O33 108.6(9) 10_656 53_666 ?
O33 Ti1 O33 40(2) 54_655 53_666 ?
O33 Ti1 O33 140(2) 6_566 53_666 ?
O33 Ti1 O33 108.6(9) 57_666 53_666 ?
O33 Ti1 O33 71.4(9) 9 53_666 ?
O33 Ti1 O33 71.4(9) 50_556 5 ?
O33 Ti1 O33 108.6(9) 2_665 5 ?
O33 Ti1 O33 108.6(9) 58_565 5 ?
O33 Ti1 O33 71.4(9) 10_656 5 ?
O33 Ti1 O33 140(2) 54_655 5 ?
O33 Ti1 O33 40(2) 6_566 5 ?
O33 Ti1 O33 71.4(9) 57_666 5 ?
O33 Ti1 O33 108.6(9) 9 5 ?
O33 Ti1 O33 180.0 53_666 5 ?
O33 Ti1 O33 40(2) 50_556 49_666 ?
O33 Ti1 O33 140(2) 2_665 49_666 ?
O33 Ti1 O33 108.6(9) 58_565 49_666 ?
O33 Ti1 O33 71.4(9) 10_656 49_666 ?
O33 Ti1 O33 71.4(9) 54_655 49_666 ?
O33 Ti1 O33 108.6(9) 6_566 49_666 ?
O33 Ti1 O33 108.6(9) 57_666 49_666 ?
O33 Ti1 O33 71.4(9) 9 49_666 ?
O33 Ti1 O33 108.6(9) 53_666 49_666 ?
O33 Ti1 O33 71.4(9) 5 49_666 ?
O33 Ti1 O33 140(2) 50_556 . ?
O33 Ti1 O33 40(2) 2_665 . ?
O33 Ti1 O33 71.4(9) 58_565 . ?
O33 Ti1 O33 108.6(9) 10_656 . ?
O33 Ti1 O33 108.6(9) 54_655 . ?
O33 Ti1 O33 71.4(9) 6_566 . ?
O33 Ti1 O33 71.4(9) 57_666 . ?
O33 Ti1 O33 108.6(9) 9 . ?
O33 Ti1 O33 71.4(9) 53_666 . ?
O33 Ti1 O33 108.6(9) 5 . ?
O33 Ti1 O33 180.0 49_666 . ?
O1 P1 O1 114.65(9) 24_665 30_466 ?
O1 P1 O1 114.65(9) 24_665 . ?
O1 P1 O1 114.65(9) 30_466 . ?
O1 P1 O2 103.59(11) 24_665 . ?
O1 P1 O2 103.59(11) 30_466 . ?
O1 P1 O2 103.59(11) . . ?
O1 P1 K1 94.89(10) 24_665 . ?
O1 P1 K1 147.80(11) 30_466 . ?
O1 P1 K1 58.51(10) . . ?
O2 P1 K1 54.55(4) . . ?
O1 P1 K1 58.51(10) 24_665 69_666 ?
O1 P1 K1 94.89(10) 30_466 69_666 ?
O1 P1 K1 147.80(11) . 69_666 ?
O2 P1 K1 54.55(4) . 69_666 ?
K1 P1 K1 89.74(6) . 69_666 ?
O1 P1 K1 147.80(11) 24_665 29_455 ?
O1 P1 K1 58.51(10) 30_466 29_455 ?
O1 P1 K1 94.89(10) . 29_455 ?
O2 P1 K1 54.55(4) . 29_455 ?
K1 P1 K1 89.74(6) . 29_455 ?
K1 P1 K1 89.74(6) 69_666 29_455 ?
F1 Na1 F1 118.34(4) 54_655 10_656 ?
F1 Na1 F1 118.34(4) 54_655 . ?
F1 Na1 F1 118.34(4) 10_656 . ?
F1 Na1 O1 65.49(9) 54_655 . ?
F1 Na1 O1 153.32(14) 10_656 . ?
F1 Na1 O1 74.72(8) . . ?
F1 Na1 O1 153.32(14) 54_655 10_656 ?
F1 Na1 O1 74.72(8) 10_656 10_656 ?
F1 Na1 O1 65.49(9) . 10_656 ?
O1 Na1 O1 92.42(10) . 10_656 ?
F1 Na1 O1 74.72(8) 54_655 7_665 ?
F1 Na1 O1 65.49(9) 10_656 7_665 ?
F1 Na1 O1 153.32(14) . 7_665 ?
O1 Na1 O1 92.41(10) . 7_665 ?
O1 Na1 O1 92.41(10) 10_656 7_665 ?
F1 Na1 O33 56.5(5) 54_655 53_666 ?
F1 Na1 O33 86.9(6) 10_656 53_666 ?
F1 Na1 O33 105.3(7) . 53_666 ?
O1 Na1 O33 113.1(5) . 53_666 ?
O1 Na1 O33 150.2(5) 10_656 53_666 ?
O1 Na1 O33 101.2(7) 7_665 53_666 ?
F1 Na1 O33 105.3(7) 54_655 9 ?
F1 Na1 O33 56.5(5) 10_656 9 ?
F1 Na1 O33 86.9(6) . 9 ?
O1 Na1 O33 150.2(5) . 9 ?
O1 Na1 O33 101.2(7) 10_656 9 ?
O1 Na1 O33 113.1(5) 7_665 9 ?
O33 Na1 O33 49.0(10) 53_666 9 ?
F1 Na1 O33 86.9(6) 54_655 2_665 ?
F1 Na1 O33 105.3(7) 10_656 2_665 ?
F1 Na1 O33 56.5(5) . 2_665 ?
O1 Na1 O33 101.2(7) . 2_665 ?
O1 Na1 O33 113.1(5) 10_656 2_665 ?
O1 Na1 O33 150.2(5) 7_665 2_665 ?
O33 Na1 O33 49.0(10) 53_666 2_665 ?
O33 Na1 O33 49.0(10) 9 2_665 ?
F1 Na1 O32 69.0(5) 54_655 54_655 ?
F1 Na1 O32 68.6(4) 10_656 54_655 ?
F1 Na1 O32 112.7(5) . 54_655 ?
O1 Na1 O32 130.6(4) . 54_655 ?
O1 Na1 O32 136.2(4) 10_656 54_655 ?
O1 Na1 O32 93.5(4) 7_665 54_655 ?
O33 Na1 O32 18.3(6) 53_666 54_655 ?
O33 Na1 O32 37.7(7) 9 54_655 ?
O33 Na1 O32 57.6(6) 2_665 54_655 ?
F1 Na1 O32 68.6(4) 54_655 2_665 ?
F1 Na1 O32 112.7(5) 10_656 2_665 ?
F1 Na1 O32 69.0(5) . 2_665 ?
O1 Na1 O32 93.5(4) . 2_665 ?
O1 Na1 O32 130.6(4) 10_656 2_665 ?
O1 Na1 O32 136.2(4) 7_665 2_665 ?
O33 Na1 O32 37.7(7) 53_666 2_665 ?
O33 Na1 O32 57.6(6) 9 2_665 ?
O33 Na1 O32 18.3(6) 2_665 2_665 ?
O32 Na1 O32 51.6(7) 54_655 2_665 ?
F1 Na1 O32 112.7(5) 54_655 9 ?
F1 Na1 O32 69.0(5) 10_656 9 ?
F1 Na1 O32 68.6(4) . 9 ?
O1 Na1 O32 136.2(4) . 9 ?
O1 Na1 O32 93.5(4) 10_656 9 ?
O1 Na1 O32 130.6(4) 7_665 9 ?
O33 Na1 O32 57.6(6) 53_666 9 ?
O33 Na1 O32 18.3(6) 9 9 ?
O33 Na1 O32 37.7(7) 2_665 9 ?
O32 Na1 O32 51.6(7) 54_655 9 ?
O32 Na1 O32 51.6(7) 2_665 9 ?
F1 K1 F1 126.09(16) . 2_665 ?
F1 K1 O31 63.04(8) . . ?
F1 K1 O31 63.04(8) 2_665 . ?
F1 K1 O32 63.59(9) . . ?
F1 K1 O32 63.59(9) 2_665 . ?
O31 K1 O32 11.2(4) . . ?
F1 K1 O32 63.59(9) . 2_665 ?
F1 K1 O32 63.59(9) 2_665 2_665 ?
O31 K1 O32 11.2(4) . 2_665 ?
O32 K1 O32 22.3(8) . 2_665 ?
F1 K1 O33 75.4(6) . . ?
F1 K1 O33 50.7(6) 2_665 . ?
O31 K1 O33 12.4(6) . . ?
O32 K1 O33 16.6(4) . . ?
O32 K1 O33 16.6(4) 2_665 . ?
F1 K1 O33 50.7(6) . 2_665 ?
F1 K1 O33 75.4(6) 2_665 2_665 ?
O31 K1 O33 12.4(6) . 2_665 ?
O32 K1 O33 16.6(4) . 2_665 ?
O32 K1 O33 16.6(4) 2_665 2_665 ?
O33 K1 O33 24.8(12) . 2_665 ?
F1 K1 O2 83.19(8) . . ?
F1 K1 O2 139.92(6) 2_665 . ?
O31 K1 O2 135.49(8) . . ?
O32 K1 O2 142.7(2) . . ?
O32 K1 O2 127.1(3) 2_665 . ?
O33 K1 O2 143.4(3) . . ?
O33 K1 O2 126.2(5) 2_665 . ?
F1 K1 O2 83.19(8) . 52_655 ?
F1 K1 O2 139.92(6) 2_665 52_655 ?
O31 K1 O2 135.49(8) . 52_655 ?
O32 K1 O2 127.1(3) . 52_655 ?
O32 K1 O2 142.7(3) 2_665 52_655 ?
O33 K1 O2 143.4(3) . 52_655 ?
O33 K1 O2 126.2(5) 2_665 52_655 ?
O2 K1 O2 59.43(10) . 52_655 ?
F1 K1 O2 139.92(6) . 2_665 ?
F1 K1 O2 83.19(8) 2_665 2_665 ?
O31 K1 O2 135.49(8) . 2_665 ?
O32 K1 O2 127.1(3) . 2_665 ?
O32 K1 O2 142.7(2) 2_665 2_665 ?
O33 K1 O2 126.2(5) . 2_665 ?
O33 K1 O2 143.4(3) 2_665 2_665 ?
O2 K1 O2 89.02(16) . 2_665 ?
O2 K1 O2 59.43(10) 52_655 2_665 ?
F1 K1 O2 139.92(6) . 51_565 ?
F1 K1 O2 83.19(8) 2_665 51_565 ?
O31 K1 O2 135.49(8) . 51_565 ?
O32 K1 O2 142.7(2) . 51_565 ?
O32 K1 O2 127.1(3) 2_665 51_565 ?
O33 K1 O2 126.2(5) . 51_565 ?
O33 K1 O2 143.4(3) 2_665 51_565 ?
O2 K1 O2 59.43(10) . 51_565 ?
O2 K1 O2 89.02(17) 52_655 51_565 ?
O2 K1 O2 59.43(10) 2_665 51_565 ?
F1 K1 O1 63.69(5) . . ?
F1 K1 O1 115.80(6) 2_665 . ?
O31 K1 O1 89.49(6) . . ?
O32 K1 O1 99.2(4) . . ?
O32 K1 O1 79.8(4) 2_665 . ?
O33 K1 O1 95.6(3) . . ?
O33 K1 O1 83.4(3) 2_665 . ?
O2 K1 O1 47.99(8) . . ?
O2 K1 O1 101.15(6) 52_655 . ?
O2 K1 O1 132.99(11) 2_665 . ?
O2 K1 O1 79.59(5) 51_565 . ?
Mn1 F1 Na1 107.76(9) . . ?
Mn1 F1 Na1 107.76(9) . 52_655 ?
Na1 F1 Na1 116.67(16) . 52_655 ?
Mn1 F1 K1 130.05(15) . . ?
Na1 F1 K1 97.51(8) . . ?
Na1 F1 K1 97.51(8) 52_655 . ?
P1 O1 Mn1 135.30(15) . 30_466 ?
P1 O1 Na1 125.68(14) . . ?
Mn1 O1 Na1 96.12(9) 30_466 . ?
P1 O1 K1 96.55(12) . . ?
Mn1 O1 K1 102.62(9) 30_466 . ?
Na1 O1 K1 85.21(9) . . ?
P1 O2 K1 99.24(8) . . ?
P1 O2 K1 99.24(8) . 69_666 ?
K1 O2 K1 117.47(4) . 69_666 ?
P1 O2 K1 99.24(8) . 29_455 ?
K1 O2 K1 117.47(4) . 29_455 ?
K1 O2 K1 117.47(4) 69_666 29_455 ?
O32 O31 O32 171(10) 2_665 . ?
O32 O31 O33 89.0(17) 2_665 . ?
O32 O31 O33 89.0(17) . . ?
O32 O31 O33 89.0(17) 2_665 2_665 ?
O32 O31 O33 89.0(17) . 2_665 ?
O33 O31 O33 156(10) . 2_665 ?
O32 O31 Ti1 85(6) 2_665 . ?
O32 O31 Ti1 85(6) . . ?
O33 O31 Ti1 78(5) . . ?
O33 O31 Ti1 78(5) 2_665 . ?
O32 O31 K1 95(6) 2_665 . ?
O32 O31 K1 95(6) . . ?
O33 O31 K1 102(5) . . ?
O33 O31 K1 102(5) 2_665 . ?
Ti1 O31 K1 180.0 . . ?
O32 O31 Na1 45.9(10) 2_665 . ?
O32 O31 Na1 135.15(19) . . ?
O33 O31 Na1 134.9(7) . . ?
O33 O31 Na1 47.7(13) 2_665 . ?
Ti1 O31 Na1 94.5(9) . . ?
K1 O31 Na1 85.5(9) . . ?
O32 O31 Na1 135.15(19) 2_665 52_655 ?
O32 O31 Na1 45.9(10) . 52_655 ?
O33 O31 Na1 134.9(7) . 52_655 ?
O33 O31 Na1 47.7(13) 2_665 52_655 ?
Ti1 O31 Na1 94.5(9) . 52_655 ?
K1 O31 Na1 85.5(9) . 52_655 ?
Na1 O31 Na1 89.64(13) . 52_655 ?
O32 O31 Na1 45.9(11) 2_665 51_565 ?
O32 O31 Na1 135.15(18) . 51_565 ?
O33 O31 Na1 47.7(13) . 51_565 ?
O33 O31 Na1 134.9(7) 2_665 51_565 ?
Ti1 O31 Na1 94.5(9) . 51_565 ?
K1 O31 Na1 85.5(9) . 51_565 ?
Na1 O31 Na1 89.64(13) . 51_565 ?
Na1 O31 Na1 171.0(17) 52_655 51_565 ?
O32 O31 Na1 135.15(18) 2_665 2_665 ?
O32 O31 Na1 45.9(11) . 2_665 ?
O33 O31 Na1 47.7(13) . 2_665 ?
O33 O31 Na1 134.9(7) 2_665 2_665 ?
Ti1 O31 Na1 94.5(9) . 2_665 ?
K1 O31 Na1 85.5(9) . 2_665 ?
Na1 O31 Na1 171.0(17) . 2_665 ?
Na1 O31 Na1 89.64(13) 52_655 2_665 ?
Na1 O31 Na1 89.64(13) 51_565 2_665 ?
O31 O32 O33 50(2) . . ?
O31 O32 O33 50(2) . 2_665 ?
O33 O32 O33 97(4) . 2_665 ?
O31 O32 O32 5(6) . 2_665 ?
O33 O32 O32 49(2) . 2_665 ?
O33 O32 O32 49(2) 2_665 2_665 ?
O31 O32 O33 140(7) . 6_566 ?
O33 O32 O33 113(3) . 6_566 ?
O33 O32 O33 113(3) 2_665 6_566 ?
O32 O32 O33 134.8(12) 2_665 6_566 ?
O31 O32 Ti1 78(6) . . ?
O33 O32 Ti1 73(2) . . ?
O33 O32 Ti1 73(2) 2_665 . ?
O32 O32 Ti1 73.4(7) 2_665 . ?
O33 O32 Ti1 61.5(12) 6_566 . ?
O31 O32 Na1 125.5(14) . 52_655 ?
O33 O32 Na1 175(2) . 52_655 ?
O33 O32 Na1 78.4(17) 2_665 52_655 ?
O32 O32 Na1 126.3(4) 2_665 52_655 ?
O33 O32 Na1 70.0(7) 6_566 52_655 ?
Ti1 O32 Na1 105.7(7) . 52_655 ?
O31 O32 Na1 125.5(13) . 2_665 ?
O33 O32 Na1 78.4(17) . 2_665 ?
O33 O32 Na1 175(2) 2_665 2_665 ?
O32 O32 Na1 126.3(4) 2_665 2_665 ?
O33 O32 Na1 70.0(7) 6_566 2_665 ?
Ti1 O32 Na1 105.7(7) . 2_665 ?
Na1 O32 Na1 106.1(7) 52_655 2_665 ?
O31 O32 K1 74(6) . . ?
O33 O32 K1 89(3) . . ?
O33 O32 K1 89(3) 2_665 . ?
O32 O32 K1 78.8(4) 2_665 . ?
O33 O32 K1 146.4(14) 6_566 . ?
Ti1 O32 K1 152.2(10) . . ?
Na1 O32 K1 90.6(5) 52_655 . ?
Na1 O32 K1 90.6(5) 2_665 . ?
O31 O33 O32 41(2) . 2_665 ?
O31 O33 O32 41(2) . . ?
O32 O33 O32 82(4) 2_665 . ?
O31 O33 O33 12(5) . 2_665 ?
O32 O33 O33 41(2) 2_665 2_665 ?
O32 O33 O33 41(2) . 2_665 ?
O31 O33 O32 147(5) . 58_565 ?
O32 O33 O32 127(3) 2_665 58_565 ?
O32 O33 O32 127(3) . 58_565 ?
O33 O33 O32 135.2(12) 2_665 58_565 ?
O31 O33 Ti1 82(5) . . ?
O32 O33 Ti1 81(2) 2_665 . ?
O32 O33 Ti1 81(2) . . ?
O33 O33 Ti1 70.2(11) 2_665 . ?
O32 O33 Ti1 65.0(12) 58_565 . ?
O31 O33 Na1 121.8(18) . 51_565 ?
O32 O33 Na1 83.3(15) 2_665 51_565 ?
O32 O33 Na1 160(3) . 51_565 ?
O33 O33 Na1 124.7(6) 2_665 51_565 ?
O32 O33 Na1 72.3(10) 58_565 51_565 ?
Ti1 O33 Na1 109.0(10) . 51_565 ?
O31 O33 Na1 121.8(18) . 2_665 ?
O32 O33 Na1 160(3) 2_665 2_665 ?
O32 O33 Na1 83.3(15) . 2_665 ?
O33 O33 Na1 124.7(6) 2_665 2_665 ?
O32 O33 Na1 72.3(10) 58_565 2_665 ?
Ti1 O33 Na1 109.0(10) . 2_665 ?
Na1 O33 Na1 108.2(11) 51_565 2_665 ?
O31 O33 K1 66(5) . . ?
O32 O33 K1 75(3) 2_665 . ?
O32 O33 K1 75(3) . . ?
O33 O33 K1 77.6(6) 2_665 . ?
O32 O33 K1 147.2(16) 58_565 . ?
Ti1 O33 K1 147.8(16) . . ?
Na1 O33 K1 89.1(7) 51_565 . ?
Na1 O33 K1 89.1(7) 2_665 . ?
 
_refine_diff_density_max    0.955
_refine_diff_density_min   -0.495
_refine_diff_density_rms    0.108

_shelxl_version_number 2013-2



